Loading in 2 Seconds...
Loading in 2 Seconds...
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author. While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
International Aircraft Materials Fire Test Working Group Meeting Development of a New Flammability Test for Magnesium-Alloy Seat Structure International Aircraft Materials Fire Test Working Group, Solothurn, Switzerland Tim Marker, FAA Technical Center June 25, 2014
Activities Since Last Meeting Refined method of determining when sample begins to burn (10-sec dwell) Refined method of determining when sample self-extinguishes (video) Investigated various techniques when measuring post-test weights Investigated use of igniterless stator for more consistent flame Experimentation with not moving sample away from burner after test Experimentation with new sample holder that allows elongation during heating Insert new test method into Handbook
Measurement of Bar and Residue Weight After 1 hour After 4 hours After 24 hours After wire-brushing After hammering!
Refinement of Burner Flame for Increased Repeatability (using Elektron-43 as the testing material) Use of Stator/Turbulator (baseline) 90% passing Use of Flame Retention Head yields only 24% passing Use of Modified Flame Retention Head yields only 79% passing Igniterless Stator 85% passing
Surface Area to Volume Ratio For truncated cone test sample: (l = 10, Db = 1.57, Dh = 0.40) Surface Area = 33.0592 in2 Volume = 8.5161 in3 SAV Ratio = 33.0592 ÷ 8.5161 = 3.88 in-1 SAV Ratio = 3.88
Surface Area to Volume Ratio For rectangular bar test sample: Surface Area = (2 x 0.25 x 20) + (2 x 1.5 x 20) + (2 x 0.25 x 1.5) Surface Area = (10) + (60) + (0.75) = 70.75 in2 Volume = (0.25 x 1.5 x 20) = 7.5 in3 SAV Ratio = 70.75 ÷ 7.5 = 9.42 in-1 SAV Ratio = 9.42
Surface Area to Volume Ratio For hollow cylinder test sample (1.75 OD, wall thickness = 0.094): Surface Area = 84.22782 in2 SAV Ratio = 84.22782 ÷ 3.90248 = 21.58 in-1 SAV Ratio = 21.58
Surface Area to Volume Ratio For thin sheet test sample: (10 inch square, thickness = 0.0625) Surface Area = (2 x 10 x 10) + (4 x 0.0625 x 10) Surface Area = (200) + (2.5) = 202.5 in2 Volume = (l x w x t) Volume = (10 x 10 x .0625) = 6.25 in3 SAV Ratio = 202.5 ÷ 6.25 = 32.4 in-1 SAV Ratio = 32.4
Surface Area to Volume Ratio For solid basketball-sized test sample: (9.5-inch diameter) Surface Area = 4 pr2 Surface Area = (4 x 3.14 x 22.5625) = 283.53 in2 Volume = 4/3pr3 Volume = (4 ÷ 3 x 3.14 x 107.17) = 448.92 in3 SAV Ratio = 283.53 ÷ 448.92 = 0.632 in-1 SAV Ratio = 0.632
Considerations for Qualifying Other Mag-Alloy Components Possible to define a maximum SAV ratio + use oil burner test For Example: If SAV ratio is less than xx, use oil burner test If SAV ratio is greater than xx, use suitable electrical arc test
Discussion Items for Inclusion in Advisory Circular Testing of coatings (powder coatings, anodizing, paints) Can other seat components also be made of magnesium alloy? Can “Equivalent Geometry” be defined using SAV ratio?